#------------------------------------------------------------------------------
#$Date: 2022-09-15 14:08:19 +0300 (Thu, 15 Sep 2022) $
#$Revision: 277870 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/10/11/7101119.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7101119
loop_
_publ_author_name
'Brandao, P.'
'Almeida Paz, Filipe A.'
'Rocha, Joao'
_publ_section_title
;
A Novel Microporous Copper Silicate:
Na2Cu2Si4O11.2H2O
;
_journal_issue                   2
_journal_name_full               'Chemical Communications'
_journal_paper_doi               10.1039/b410731d
_journal_year                    2005
_chemical_formula_moiety         'Cu2 H4 O13 Si4, 2(Na)'
_chemical_formula_sum            'Cu2 H4 Na2 O13 Si4'
_chemical_formula_weight         497.45
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             '17th May, 2004'
_audit_creation_method           'SHELXL-97 plus manual editing'
_cell_angle_alpha                101.107(2)
_cell_angle_beta                 94.340(2)
_cell_angle_gamma                102.480(2)
_cell_formula_units_Z            1
_cell_length_a                   5.2228(7)
_cell_length_b                   6.4109(9)
_cell_length_c                   8.5169(12)
_cell_measurement_reflns_used    1941
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.21
_cell_measurement_theta_min      2.46
_cell_volume                     271.16(7)
_computing_cell_refinement       'SAINT+ (Bruker AXS)'
_computing_data_collection       'SMART (Bruker AXS)'
_computing_data_reduction        'SAINT+ (Bruker AXS)'
_computing_molecular_graphics    'SHELXTL (Bruker 2001)'
_computing_publication_material  'SHELXTL (Bruker 2001)'
_computing_structure_refinement  'SHELXTL (Bruker 2001)'
_computing_structure_solution    'SIR-92 (Altomare at al. 1994)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Smart-CCD-1000 BRUKER'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0233
_diffrn_reflns_av_sigmaI/netI    0.0216
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            3412
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         3.69
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    4.520
_exptl_absorpt_correction_T_max  0.873
_exptl_absorpt_correction_T_min  0.530
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS: G.M.Sheldrick, (1996) University of Gottingen, Germany
;
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    3.046
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Needle
_exptl_crystal_F_000             244
_exptl_crystal_size_max          0.57
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.484
_refine_diff_density_min         -0.418
_refine_diff_density_rms         0.106
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.066
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     103
_refine_ls_number_reflns         1099
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.064
_refine_ls_R_factor_all          0.0292
_refine_ls_R_factor_gt           0.0233
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0256P)²+0.6257P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0581
_refine_ls_wR_factor_ref         0.0610
_reflns_number_gt                948
_reflns_number_total             1099
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            b410731d.txt
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               7101119
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cu1 Cu 1.29574(7) 1.11304(6) 0.06820(4) 0.00894(13) Uani 1 1 d .
Si1 Si 0.96324(16) 0.88020(13) 0.31186(9) 0.00738(19) Uani 1 1 d .
Si2 Si 0.38272(15) 0.66252(13) 0.16871(9) 0.00705(19) Uani 1 1 d .
O1 O 1.0031(4) 1.0419(4) 0.1915(3) 0.0132(5) Uani 1 1 d .
O2 O 1.0000 1.0000 0.5000 0.0167(7) Uani 1 2 d S
O3 O 1.1785(4) 0.7273(3) 0.3007(2) 0.0099(4) Uani 1 1 d .
O4 O 0.6730(4) 0.7108(3) 0.2753(2) 0.0111(4) Uani 1 1 d .
O5 O 0.3909(4) 0.8271(3) 0.0453(2) 0.0092(4) Uani 1 1 d .
O6 O 0.2682(4) 0.4116(3) 0.0906(3) 0.0122(5) Uani 1 1 d .
Na1 Na 0.8611(2) 0.3640(2) 0.20223(15) 0.0156(3) Uani 1 1 d .
O1W O 0.5770(5) 0.2703(5) 0.3898(3) 0.0305(6) Uani 1 1 d D
H1 H 0.638(8) 0.243(8) 0.475(3) 0.046 Uiso 1 1 d D
H2 H 0.428(5) 0.295(8) 0.399(5) 0.046 Uiso 1 1 d D
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 Cu1 O1 92.63(9) 1_665 . no
O6 Cu1 O5 90.65(9) 1_665 2_775 no
O1 Cu1 O5 175.12(9) . 2_775 no
O6 Cu1 O5 169.97(9) 1_665 1_655 no
O1 Cu1 O5 95.88(9) . 1_655 no
O5 Cu1 O5 80.54(9) 2_775 1_655 no
O6 Cu1 Cu1 130.88(7) 1_665 2_875 no
O1 Cu1 Cu1 135.92(7) . 2_875 no
O5 Cu1 Cu1 40.41(6) 2_775 2_875 no
O5 Cu1 Cu1 40.13(6) 1_655 2_875 no
O6 Cu1 Na1 78.30(7) 1_665 1_665 no
O1 Cu1 Na1 126.77(7) . 1_665 no
O5 Cu1 Na1 50.52(7) 2_775 1_665 no
O5 Cu1 Na1 92.31(7) 1_655 1_665 no
Cu1 Cu1 Na1 67.11(3) 2_875 1_665 no
O6 Cu1 Na1 47.45(7) 1_665 1_565 no
O1 Cu1 Na1 46.03(7) . 1_565 no
O5 Cu1 Na1 137.73(6) 2_775 1_565 no
O5 Cu1 Na1 141.70(6) 1_655 1_565 no
Cu1 Cu1 Na1 177.75(3) 2_875 1_565 no
Na1 Cu1 Na1 112.88(4) 1_665 1_565 no
O6 Cu1 Na1 140.56(7) 1_665 2_765 no
O1 Cu1 Na1 95.71(7) . 2_765 no
O5 Cu1 Na1 84.01(6) 2_775 2_765 no
O5 Cu1 Na1 43.68(6) 1_655 2_765 no
Cu1 Cu1 Na1 57.08(3) 2_875 2_765 no
Na1 Cu1 Na1 124.20(2) 1_665 2_765 no
Na1 Cu1 Na1 122.88(2) 1_565 2_765 no
O1 Si1 O2 114.50(9) . . no
O1 Si1 O4 112.70(12) . . no
O2 Si1 O4 106.70(9) . . no
O1 Si1 O3 112.09(11) . . no
O2 Si1 O3 104.27(8) . . no
O4 Si1 O3 105.85(11) . . no
O1 Si1 Na1 123.90(9) . . no
O2 Si1 Na1 121.45(4) . . no
O4 Si1 Na1 55.00(8) . . no
O3 Si1 Na1 51.21(8) . . no
O6 Si2 O5 115.59(12) . . no
O6 Si2 O4 112.72(12) . . no
O5 Si2 O4 110.09(11) . . no
O6 Si2 O3 105.35(11) . 1_455 no
O5 Si2 O3 106.85(11) . 1_455 no
O4 Si2 O3 105.44(11) . 1_455 no
O6 Si2 Na1 50.72(8) . 1_455 no
O5 Si2 Na1 119.90(8) . 1_455 no
O4 Si2 Na1 129.58(9) . 1_455 no
O3 Si2 Na1 55.25(8) 1_455 1_455 no
O6 Si2 Na1 73.58(9) . 2_665 no
O4 Si2 Na1 138.72(9) . 2_665 no
O3 Si2 Na1 112.07(8) 1_455 2_665 no
Na1 Si2 Na1 87.20(4) 1_455 2_665 no
O6 Si2 Na1 68.75(9) . . no
O5 Si2 Na1 122.16(8) . . no
O4 Si2 Na1 45.32(8) . . no
O3 Si2 Na1 128.39(8) 1_455 . no
Na1 Si2 Na1 106.11(4) 1_455 . no
Na1 Si2 Na1 114.44(3) 2_665 . no
Si1 O1 Cu1 128.99(13) . . no
Si1 O1 Na1 128.43(12) . 1_565 no
Cu1 O1 Na1 97.08(9) . 1_565 no
Si1 O2 Si1 180.0 . 2_776 no
Si1 O3 Si2 134.82(13) . 1_655 no
Si1 O3 Na1 98.02(10) . . no
Si2 O3 Na1 91.59(9) 1_655 . no
Si1 O4 Si2 141.97(14) . . no
Si1 O4 Na1 94.17(10) . . no
Si2 O4 Na1 108.06(11) . . no
Si2 O5 Cu1 118.45(11) . 2_775 no
Si2 O5 Cu1 130.71(12) . 1_455 no
Cu1 O5 Cu1 99.46(9) 2_775 1_455 no
Si2 O5 Na1 109.22(11) . 2_665 no
Cu1 O5 Na1 89.41(8) 2_775 2_665 no
Cu1 O5 Na1 100.92(9) 1_455 2_665 no
Si2 O6 Cu1 149.34(14) . 1_445 no
Si2 O6 Na1 98.31(10) . 1_455 no
Cu1 O6 Na1 95.96(9) 1_445 1_455 no
O1 Na1 O1W 90.49(10) 1_545 . no
O1 Na1 O5 83.66(8) 1_545 2_665 no
O1W Na1 O5 102.44(10) . 2_665 no
O1 Na1 O6 72.88(8) 1_545 1_655 no
O1W Na1 O6 155.37(10) . 1_655 no
O5 Na1 O6 93.83(8) 2_665 1_655 no
O1 Na1 O3 120.47(9) 1_545 . no
O1W Na1 O3 113.02(10) . . no
O5 Na1 O3 135.59(9) 2_665 . no
O6 Na1 O3 63.83(8) 1_655 . no
O1 Na1 O4 167.44(9) 1_545 . no
O1W Na1 O4 77.89(9) . . no
O5 Na1 O4 103.32(8) 2_665 . no
O6 Na1 O4 116.43(8) 1_655 . no
O3 Na1 O4 61.44(7) . . no
O1 Na1 Si2 98.45(7) 1_545 1_655 no
O1W Na1 Si2 142.90(9) . 1_655 no
O5 Na1 Si2 114.26(7) 2_665 1_655 no
O6 Na1 Si2 30.97(5) 1_655 1_655 no
O3 Na1 Si2 33.16(5) . 1_655 no
O4 Na1 Si2 88.26(6) . 1_655 no
O1 Na1 Cu1 92.10(7) 1_545 1_445 no
O1W Na1 Cu1 63.23(8) . 1_445 no
O5 Na1 Cu1 40.07(5) 2_665 1_445 no
O6 Na1 Cu1 133.54(7) 1_655 1_445 no
O3 Na1 Cu1 147.43(7) . 1_445 no
O4 Na1 Cu1 86.94(6) . 1_445 no
Si2 Na1 Cu1 151.00(5) 1_655 1_445 no
O1 Na1 Si1 150.51(8) 1_545 . no
O1W Na1 Si1 97.97(9) . . no
O5 Na1 Si1 121.40(7) 2_665 . no
O6 Na1 Si1 88.93(6) 1_655 . no
O3 Na1 Si1 30.77(5) . . no
O4 Na1 Si1 30.83(5) . . no
Si2 Na1 Si1 58.74(3) 1_655 . no
Cu1 Na1 Si1 116.96(4) 1_445 . no
O1 Na1 Cu1 36.89(5) 1_545 1_545 no
O1W Na1 Cu1 126.73(9) . 1_545 no
O5 Na1 Cu1 83.48(6) 2_665 1_545 no
O6 Na1 Cu1 36.59(5) 1_655 1_545 no
O3 Na1 Cu1 95.26(6) . 1_545 no
O4 Na1 Cu1 153.01(7) . 1_545 no
Si2 Na1 Cu1 65.44(3) 1_655 1_545 no
Cu1 Na1 Cu1 112.88(4) 1_445 1_545 no
Si1 Na1 Cu1 124.10(4) . 1_545 no
O1 Na1 Si2 104.71(7) 1_545 2_665 no
O1W Na1 Si2 119.70(8) . 2_665 no
O5 Na1 Si2 27.92(5) 2_665 2_665 no
O6 Na1 Si2 82.79(6) 1_655 2_665 no
O3 Na1 Si2 108.04(6) . 2_665 no
O4 Na1 Si2 85.44(6) . 2_665 no
Si2 Na1 Si2 92.80(4) 1_655 2_665 no
Cu1 Na1 Si2 58.32(3) 1_445 2_665 no
Si1 Na1 Si2 95.52(4) . 2_665 no
Cu1 Na1 Si2 89.75(3) 1_545 2_665 no
O1 Na1 Cu1 48.28(6) 1_545 2_765 no
O1W Na1 Cu1 98.80(9) . 2_765 no
O5 Na1 Cu1 35.40(5) 2_665 2_765 no
O6 Na1 Cu1 83.80(6) 1_655 2_765 no
O3 Na1 Cu1 147.09(7) . 2_765 no
O4 Na1 Cu1 137.67(7) . 2_765 no
Si2 Na1 Cu1 114.01(4) 1_655 2_765 no
Cu1 Na1 Cu1 55.80(2) 1_445 2_765 no
Si1 Na1 Cu1 154.39(5) . 2_765 no
Cu1 Na1 Cu1 57.12(2) 1_545 2_765 no
Si2 Na1 Cu1 59.26(3) 2_665 2_765 no
Na1 O1W H1 119(3) . . no
Na1 O1W H2 128(3) . . no
H1 O1W H2 110(2) . . no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cu1 O6 1.924(2) 1_665 no
Cu1 O1 1.942(2) . no
Cu1 O5 1.967(2) 2_775 no
Cu1 O5 1.979(2) 1_655 no
Cu1 Cu1 3.0109(7) 2_875 no
Cu1 Na1 3.0559(14) 1_665 no
Cu1 Na1 3.2109(13) 1_565 no
Cu1 Na1 3.3538(14) 2_765 no
Si1 O1 1.587(2) . no
Si1 O2 1.6155(8) . no
Si1 O4 1.631(2) . no
Si1 O3 1.640(2) . no
Si1 Na1 3.1745(15) . no
Si2 O6 1.581(2) . no
Si2 O5 1.623(2) . no
Si2 O4 1.643(2) . no
Si2 O3 1.663(2) 1_455 no
Si2 Na1 3.0400(16) 1_455 no
Si2 Na1 3.2744(15) 2_665 no
Si2 Na1 3.4861(16) . no
O1 Na1 2.329(2) 1_565 no
O2 Si1 1.6155(8) 2_776 no
O3 Si2 1.663(2) 1_655 no
O3 Na1 2.499(2) . no
O4 Na1 2.607(2) . no
O5 Cu1 1.967(2) 2_775 no
O5 Cu1 1.979(2) 1_455 no
O5 Na1 2.359(2) 2_665 no
O6 Cu1 1.924(2) 1_445 no
O6 Na1 2.378(2) 1_455 no
Na1 O1 2.329(2) 1_545 no
Na1 O1W 2.336(3) . no
Na1 O5 2.359(2) 2_665 no
Na1 O6 2.378(2) 1_655 no
Na1 Si2 3.0400(16) 1_655 no
Na1 Cu1 3.0559(13) 1_445 no
Na1 Cu1 3.2109(13) 1_545 no
Na1 Si2 3.2744(15) 2_665 no
Na1 Cu1 3.3538(14) 2_765 no
O1W H1 0.84(3) . no
O1W H2 0.84(3) . no
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O1W H1 O3 0.84(3) 2.025(18) 2.836(3) 163(5) 2_766
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Si1 O1 Cu1 106.98(15) . . no
O4 Si1 O1 Cu1 -130.82(16) . . no
O3 Si1 O1 Cu1 -11.5(2) . . no
Na1 Si1 O1 Cu1 -68.72(19) . . no
O2 Si1 O1 Na1 -40.64(18) . 1_565 no
O4 Si1 O1 Na1 81.56(18) . 1_565 no
O3 Si1 O1 Na1 -159.15(14) . 1_565 no
Na1 Si1 O1 Na1 143.66(12) . 1_565 no
O6 Cu1 O1 Si1 -145.01(17) 1_665 . no
O5 Cu1 O1 Si1 29.67(18) 1_655 . no
Cu1 Cu1 O1 Si1 26.6(2) 2_875 . no
Na1 Cu1 O1 Si1 -67.67(19) 1_665 . no
Na1 Cu1 O1 Si1 -155.0(2) 1_565 . no
Na1 Cu1 O1 Si1 73.59(17) 2_765 . no
O6 Cu1 O1 Na1 9.98(10) 1_665 1_565 no
O5 Cu1 O1 Na1 -175.34(9) 1_655 1_565 no
Cu1 Cu1 O1 Na1 -178.43(4) 2_875 1_565 no
Na1 Cu1 O1 Na1 87.33(9) 1_665 1_565 no
Na1 Cu1 O1 Na1 -131.42(6) 2_765 1_565 no
O1 Si1 O3 Si2 -16.2(2) . 1_655 no
O2 Si1 O3 Si2 -140.56(16) . 1_655 no
O4 Si1 O3 Si2 107.08(19) . 1_655 no
Na1 Si1 O3 Si2 100.3(2) . 1_655 no
O1 Si1 O3 Na1 -116.50(11) . . no
O2 Si1 O3 Na1 119.10(7) . . no
O4 Si1 O3 Na1 6.74(12) . . no
O1 Si1 O4 Si2 -10.3(3) . . no
O2 Si1 O4 Si2 116.2(2) . . no
O3 Si1 O4 Si2 -133.1(2) . . no
Na1 Si1 O4 Si2 -126.7(3) . . no
O1 Si1 O4 Na1 116.44(11) . . no
O2 Si1 O4 Na1 -117.07(7) . . no
O3 Si1 O4 Na1 -6.41(11) . . no
O6 Si2 O4 Si1 137.6(2) . . no
O5 Si2 O4 Si1 6.9(3) . . no
O3 Si2 O4 Si1 -108.0(2) 1_455 . no
Na1 Si2 O4 Si1 -165.36(17) 1_455 . no
Na1 Si2 O4 Si1 46.9(3) 2_665 . no
Na1 Si2 O4 Si1 122.8(3) . . no
O6 Si2 O4 Na1 14.86(14) . . no
O5 Si2 O4 Na1 -115.81(11) . . no
O3 Si2 O4 Na1 129.27(10) 1_455 . no
Na1 Si2 O4 Na1 71.88(12) 1_455 . no
Na1 Si2 O4 Na1 -75.84(14) 2_665 . no
O6 Si2 O5 Cu1 -87.83(15) . 2_775 no
O4 Si2 O5 Cu1 41.31(16) . 2_775 no
O3 Si2 O5 Cu1 155.32(12) 1_455 2_775 no
Na1 Si2 O5 Cu1 -145.53(9) 1_455 2_775 no
Na1 Si2 O5 Cu1 -100.16(15) 2_665 2_775 no
Na1 Si2 O5 Cu1 -7.82(16) . 2_775 no
O6 Si2 O5 Cu1 136.70(15) . 1_455 no
O4 Si2 O5 Cu1 -94.16(17) . 1_455 no
O3 Si2 O5 Cu1 19.85(19) 1_455 1_455 no
Na1 Si2 O5 Cu1 79.00(16) 1_455 1_455 no
Na1 Si2 O5 Cu1 124.4(2) 2_665 1_455 no
Na1 Si2 O5 Cu1 -143.29(11) . 1_455 no
O6 Si2 O5 Na1 12.33(15) . 2_665 no
O4 Si2 O5 Na1 141.46(11) . 2_665 no
O3 Si2 O5 Na1 -104.52(11) 1_455 2_665 no
Na1 Si2 O5 Na1 -45.37(13) 1_455 2_665 no
Na1 Si2 O5 Na1 92.34(10) . 2_665 no
O5 Si2 O6 Cu1 134.3(2) . 1_445 no
O4 Si2 O6 Cu1 6.5(3) . 1_445 no
O3 Si2 O6 Cu1 -108.0(3) 1_455 1_445 no
Na1 Si2 O6 Cu1 -116.9(3) 1_455 1_445 no
Na1 Si2 O6 Cu1 143.0(3) 2_665 1_445 no
Na1 Si2 O6 Cu1 17.8(2) . 1_445 no
O5 Si2 O6 Na1 -108.80(11) . 1_455 no
O4 Si2 O6 Na1 123.36(11) . 1_455 no
O3 Si2 O6 Na1 8.89(12) 1_455 1_455 no
Na1 Si2 O6 Na1 -100.09(8) 2_665 1_455 no
Na1 Si2 O6 Na1 134.64(10) . 1_455 no
Si1 O3 Na1 O1 -170.34(10) . 1_545 no
Si2 O3 Na1 O1 53.94(12) 1_655 1_545 no
Si1 O3 Na1 O1W -65.22(13) . . no
Si2 O3 Na1 O1W 159.06(10) 1_655 . no
Si1 O3 Na1 O5 74.98(14) . 2_665 no
Si2 O3 Na1 O5 -60.75(14) 1_655 2_665 no
Si1 O3 Na1 O6 141.70(12) . 1_655 no
Si2 O3 Na1 O6 5.97(8) 1_655 1_655 no
Si1 O3 Na1 O4 -4.61(8) . . no
Si2 O3 Na1 O4 -140.34(11) 1_655 . no
Si1 O3 Na1 Si2 135.72(14) . 1_655 no
Si1 O3 Na1 Cu1 10.66(18) . 1_445 no
Si2 O3 Na1 Cu1 -125.06(12) 1_655 1_445 no
Si2 O3 Na1 Si1 -135.72(14) 1_655 . no
Si1 O3 Na1 Cu1 161.02(8) . 1_545 no
Si2 O3 Na1 Cu1 25.30(8) 1_655 1_545 no
Si1 O3 Na1 Si2 69.57(10) . 2_665 no
Si2 O3 Na1 Si2 -66.15(9) 1_655 2_665 no
Si1 O3 Na1 Cu1 130.47(11) . 2_765 no
Si2 O3 Na1 Cu1 -5.25(17) 1_655 2_765 no
Si1 O4 Na1 O1 106.8(4) . 1_545 no
Si2 O4 Na1 O1 -104.5(4) . 1_545 no
Si1 O4 Na1 O1W 129.51(11) . . no
Si2 O4 Na1 O1W -81.79(12) . . no
Si1 O4 Na1 O5 -130.38(10) . 2_665 no
Si2 O4 Na1 O5 18.33(13) . 2_665 no
Si1 O4 Na1 O6 -29.17(13) . 1_655 no
Si2 O4 Na1 O6 119.54(11) . 1_655 no
Si1 O4 Na1 O3 4.61(8) . . no
Si2 O4 Na1 O3 153.31(13) . . no
Si1 O4 Na1 Si2 -15.84(9) . 1_655 no
Si2 O4 Na1 Si2 132.87(10) . 1_655 no
Si1 O4 Na1 Cu1 -167.23(9) . 1_445 no
Si2 O4 Na1 Cu1 -18.52(10) . 1_445 no
Si2 O4 Na1 Si1 148.71(17) . . no
Si1 O4 Na1 Cu1 -28.38(19) . 1_545 no
Si2 O4 Na1 Cu1 120.33(14) . 1_545 no
Si1 O4 Na1 Si2 -108.79(8) . 2_665 no
Si2 O4 Na1 Si2 39.92(10) . 2_665 no
Si1 O4 Na1 Cu1 -140.67(8) . 2_765 no
Si2 O4 Na1 Cu1 8.04(16) . 2_765 no
O1 Si1 Na1 O1 109.44(19) . 1_545 no
O2 Si1 Na1 O1 -65.97(16) . 1_545 no
O4 Si1 Na1 O1 -154.99(18) . 1_545 no
O3 Si1 Na1 O1 17.08(17) . 1_545 no
O1 Si1 Na1 O1W -145.19(13) . . no
O2 Si1 Na1 O1W 39.40(9) . . no
O4 Si1 Na1 O1W -49.62(12) . . no
O3 Si1 Na1 O1W 122.46(12) . . no
O1 Si1 Na1 O5 -35.29(14) . 2_665 no
O2 Si1 Na1 O5 149.30(8) . 2_665 no
O4 Si1 Na1 O5 60.28(12) . 2_665 no
O3 Si1 Na1 O5 -127.64(13) . 2_665 no
O1 Si1 Na1 O6 58.55(12) . 1_655 no
O2 Si1 Na1 O6 -116.87(7) . 1_655 no
O4 Si1 Na1 O6 154.12(12) . 1_655 no
O3 Si1 Na1 O6 -33.81(11) . 1_655 no
O1 Si1 Na1 O3 92.35(14) . . no
O2 Si1 Na1 O3 -83.06(10) . . no
O4 Si1 Na1 O3 -172.08(14) . . no
O1 Si1 Na1 O4 -95.57(14) . . no
O2 Si1 Na1 O4 89.02(10) . . no
O3 Si1 Na1 O4 172.08(14) . . no
O1 Si1 Na1 Si2 65.82(11) . 1_655 no
O2 Si1 Na1 Si2 -109.59(5) . 1_655 no
O4 Si1 Na1 Si2 161.39(10) . 1_655 no
O3 Si1 Na1 Si2 -26.53(9) . 1_655 no
O1 Si1 Na1 Cu1 -81.23(11) . 1_445 no
O2 Si1 Na1 Cu1 103.36(6) . 1_445 no
O4 Si1 Na1 Cu1 14.34(10) . 1_445 no
O3 Si1 Na1 Cu1 -173.59(11) . 1_445 no
O1 Si1 Na1 Cu1 69.33(12) . 1_545 no
O2 Si1 Na1 Cu1 -106.08(6) . 1_545 no
O4 Si1 Na1 Cu1 164.90(11) . 1_545 no
O3 Si1 Na1 Cu1 -23.02(10) . 1_545 no
O1 Si1 Na1 Si2 -24.11(11) . 2_665 no
O2 Si1 Na1 Si2 160.48(4) . 2_665 no
O4 Si1 Na1 Si2 71.46(9) . 2_665 no
O3 Si1 Na1 Si2 -116.46(10) . 2_665 no
O1 Si1 Na1 Cu1 -14.68(16) . 2_765 no
O2 Si1 Na1 Cu1 169.91(9) . 2_765 no
O4 Si1 Na1 Cu1 80.89(14) . 2_765 no
O3 Si1 Na1 Cu1 -107.03(14) . 2_765 no
